Uni‐Mould™ Universal Moulding System
Uni‐Mould™ Advantages Traditionally, moulds made using polyester resin and gel coat are unsuitable for use as moulds for epoxy‐based parts due to well‐known release problems when used in this combination. Most polyester moulds also suffer from distortion (pulling), particularly on larger moulds, and cannot be used at elevated temperatures, making them unsuitable for in‐mould post‐curing or for pre‐pregs. Alternatives to low‐cost polyester moulds such as Advantages epoxy resin/gel coat or pre‐preg moulds can be Low cost system ideal for all medium more difficult to produce and the considerably higher material costs can be prohibitive for larger to large moulds moulds. Epoxy and polyester compatible Suitable for pre‐pregs* Uni‐Mould is different. It features unique vinylester chemistry which is 100% compatible High dimensional stability with epoxy, vinylester, polyester and pre‐pregs Long‐life moulds making it a genuinely universal tooling system. Its specially formulated resin systems are designed to Highly polishable hard‐wearing mould be dimensionally stable up to 90°C (the curing surface temperature of many pre‐preg systems) and will No special equipment or processing not pull as they cure resulting in more required dimensionally accurate moulds that will not distort for the rest of their working lives. *Out‐of autoclave use only. Pre‐pregs can be cured in Uni‐ Mould moulds up to 90°C. Moulds made using Uni‐Mould are highly polishable and, in combination with a chemical release agent (such as Easy‐Lease), will result in high‐gloss parts straight out of the mould, time after time. Uni‐Mould is designed to be used with low‐cost emulsion bound glass chopped strand mat (CSM) reinforcement which breaks down excellently in the resin, just like it would with a polyester resin, meaning that it is an ideal and cost‐effective way to create medium to large moulds.
The Uni‐Mould™ System The Uni‐Mould system is made up of 3 specially formulated resins, all capable of high operating temperatures and filled for zero shrinkage: Uni‐Mould Tooling Gel Coat (single or double application to 0.8mm) Uni‐Mould Coupling Coat (used with 1 layer of 150g CSM) Uni‐Mould Tooling Resin (used with 4 layers of 450g CSM)
Application Guide This step‐by‐step application guide assumes that your pattern or master is made from a suitable material, is fully cured, sealed and prepared with a suitable release agent. The guide assumes a mould of 1‐2sqm. For larger moulds (up to the size of full boat hulls) the Uni‐Mould system is still ideal but special measures need to be undertaken when applying the mould reinforcement. Please contact us for more details.
Uni‐Mould Tooling Gel Coat Application Uni‐Mould Tooling Gel Coat should be catalysed at 1.5‐2% using standard MEKP catalyst. Before application allow the catalysed gel coat to stand for a few minutes to settle and de‐ gas. Gel coat should be applied in two applications. For the first application aim for a consistent thickness of 0.3–0.4mm. Allow the first application to cure for around 2‐3hrs (at 20°C room temperature) before applying the second coat of gel coat, again aiming for a thickness of 0.3 ‐ 0.4mm. Allow the gel coat to cure for a minimum of 4hrs (at 20°C room temperature), preferably overnight.
Uni‐Mould Coupling Coat Application
The Uni‐Mould Coupling Coat is designed to eliminate print‐through of the mould reinforcement, to reduce the risk of blisters underneath the gel coat by ensuring the gel is reinforced with a skin of resin and glass and to provide an ideal substrate for the main reinforcement. Uni‐Mould Coupling Coat should be catalysed with standard MEKP at 1.5 – 2%. Apply a layer of the coupling coat over the mould surface and then add a single layer of 150g CSM. We do not recommend the use of glass surface tissue in lieu of the 150gsm CSM. Wet out the CSM thoroughly with the coupling coat resin and ensure that all air is removed from the reinforcement, that it is well wetted through and that the reinforcement is conforming to all the contours of the mould, particularly any tight corners.
Uni‐Mould Tooling Resin Application
The laminating technique for the Uni‐Mould Tooling Resin is quite different from conventional polyester laminating resins and it is essential that you familiarise yourself with this technique and follow the guidelines carefully in order for the resin to cure properly and result in a successful mould.
Uni‐Mould Tooling Resin is cured by its own exotherm and must reach a temperature of 50‐60°C during its cure in order to achieve its full properties. In order for this to happen your workshop environment needs to be between 18°C and 25°C and you must lay down a minimum of 4 layers of 450gsm or resin‐ rich (4:1) CSM onto the back of the mould in a single session.
Preparation In order to ensure that all the reinforcement can be laid down in a single session it is important to prepare the resin and reinforcement in advance before starting to laminate. Cut your 450gsm CSM to the right shapes for your mould, allowing for a minimum of 4 layers of mat. Once you have cut the mat, weigh it to see how much CSM you will be using. Next, weigh out 4 times the weight of the glass in resin (Uni‐Mould Tooling Resin should be used at a typical 4:1 ratio or resin to glass) which means if you are using 5kgs of CSM to reinforce your mould you should prepare 20kgs of resin.
Begin Laminating When you are ready, catalyse the resin using MEKP catalyst at 0.75 – 1.25% (depending on the ambient temperature) and mix thoroughly. Working quickly, apply resin all over the mould and then add layers of glass one at a time, wetting with plenty of resin (4:1 by weight) until you have added all the layers of glass to the back of the mould. You should use the last of the prepared resin as you add the last layer of CSM. As the laminate starts to cure the temperature will rise to 50‐60°C and the colour of the laminate will change from a mid brown to a light brown colour. Allow the resin to cure fully for 24hrs.
Post Curing For ambient temperature use, a post cure of the mould is recommended, but not required. If you intend to use the mould for pre‐preg or in‐mould post curing of your parts then an elevated temperature post cure is required. Recommended post‐cure for elevated temperature mould use: 10hrs at 60°C 2hrs at 70°C 2hrs at 80°C 2hrs at 80°C
Finished Use Composite moulds made from the Uni‐Mould system can be used for wet‐lay, vacuum bagging, resin infusion and even pre‐preg production. Moulds made from Uni‐Mould are 100% compatible with epoxy resin, polyester resin and vinylester resin.
Polishing Moulds made using Uni‐ Mould are highly polishable to a full gloss and can easily be restored if they are subject to light scratches using a composites polishing compound (such as Mirka T10). After polishing, ensure a thorough re‐application of release agent before use.
Release Agent Because Uni‐Mould’s tooling gel coat is fully compatible with epoxy, polyester, vinylester and pre‐pregs, a wide range of release agents (waxes and chemical release agents) should all result in a good release. Uni‐Mould is tested and recommended for use with Easy‐Lease Chemical Release Agent which is universally suitable for all resin systems and processes.
adaxvdvs sdf sdf3f 3